Rapid large-scale preparation of ZnO nanowires for photocatalytic application
© Ma et al; licensee Springer. 2011
Received: 31 August 2011
Accepted: 3 October 2011
Published: 3 October 2011
ZnO nanowires are a promising nanomaterial for applications in the fields of photocatalysis, nano-optoelectronics, and reinforced composite materials. However, the challenge of producing large-scale ZnO nanowires has stunted the development and practical utilization of ZnO nanowires. In this study, a modified carbothermal reduction method for preparing large-scale ZnO nanowires in less than 5 min is reported. The preparation was performed in a quartz tube furnace at atmospheric pressure without using any catalysts. A mixed gas of air and N2 with a volume ratio of 45:1 was used as the reactive and carrier gas. About 0.8 g ZnO nanowires was obtained using 1 g ZnO and 1 g graphite powder as source materials. The obtained nanowires exhibited a hexagonal wurtzite crystal structure with an average diameter of about 33 nm. Good photocatalytic activity of the nanowires toward the photodegradation of methylene blue dye under UV irradiation was also demonstrated.
Organic dyes widely used in rubber, textiles, and plastics industries are one of the largest groups of pollutants released into wastewaters . They have caused severe environmental contamination because of potential toxicity of the dyes and their visibility in water bodies. Degradation and removal of them are a vital matter for protecting the environment. However, the traditional techniques for treating organic dyes are usually non-destructive, ineffective, and costly or just transfer pollutions from water to another phase .
Recently, it has been reported that ZnO can be an alternative to conventional treatments for removing dye pollutants from water . ZnO, with a lower cost, absorbs over a larger fraction of UV spectrum and absorbs more light quanta than TiO2 . When an appropriate light source illuminates ZnO, electron/hole pairs will be produced with electrons absorbing the light energy, transitioning to the conduction band and leaving positive holes in the valence band . The produced electron/hole pairs induce a complex series of reactions that might lead to the complete degradation of the dye pollutants adsorbed on the semiconductor surface. Specifically, ZnO nanowires have demonstrated excellent photocatalytic activity because of their larger surface area and higher surface state .
Until now, there are various techniques, such as chemical vapor deposition , physical vapor deposition , electrodeposition [9, 10], and thermal evaporation  that can be used to synthesize ZnO nanowires. These methods have made great contribution to the development of ZnO-based nanoelectronic devices, such as solar cells , light-emitting diodes , field-effect transistors , field-emission displays , and biosensors . However, for employing ZnO nanowires as photocatalysts, massive ZnO nanowires are needed for practical utilization. Thus, it is necessary to develop a method to fabricate large-scale ZnO nanowires.
In this report, a modified carbothermal reduction method was developed and employed to fabricate large-scale ZnO nanowires. The fabrication process took less than 5 min. The surface morphology, microstructure, crystal structure, and optical properties of the prepared ZnO nanowires were characterized. In addition, the photocatalytic activity of the ZnO nanowires was also evaluated using methylene blue (MB) as a model dye.
Preparation of ZnO nanowires
A quartz tube furnace with an inner diameter of 7.5 cm was first heated to 1150°C. Then, the furnace was purged with a mixed gas of air (0.1 L/min) and N2 gas (4.5 L/min) continuously. Subsequently, mixtures of ZnO (Sinopharm Chemical Reagent Co., Ltd) and graphite (325 mesh) powder (2 g) with a weight ratio of 1:1, which was grounded in an agate mortar beforehand, were transferred to a quartz boat, and then the boat was placed in the middle of the furnace. After about 1 min, white snowflake-like product was carried out by the carrier gas. A 5000-mL flask, covered at the downstream of the quartz tube furnace, was used to collect the prepared product. The total reaction time was about 5 min. A white layer of products was deposited on the inner surface of the flask lastly. The weight of the obtained ZnO nanowires was about 0.8 g, which is 80% of the source ZnO powder.
The crystal structure of the prepared ZnO nanowires was analyzed using X-ray diffraction (XRD, D/max-2200/PC, Rigaku). The morphology and microstructure of the nanowires were characterized using scanning electron microscopy (SEM, Ultra 55, Carl Zeiss) and transmission electron microscopy (TEM, JEM-2100, JEOL). The chemical composition of the nanowires was analyzed by the energy dispersive X-rays spectroscopy (EDS) with the SEM. The Raman signals of the ZnO nanowires were recorded using an Ar+ ion laser as the excitation (514.5 nm) at room temperature (French Labrum-HR). The photoluminescence (PL) spectra of the ZnO nanowires were performed using a He-Cd laser line of 325 nm as an excitation source (Jobin Yvon LabRAM HR 800UV).
The photocatalytic activity of the prepared ZnO nanowires was studied by using MB as a model dye. The prepared ZnO nanowires (20 mg) were dispersed in 100 mL of MB aqueous solution (10 mg/L). Before irradiating, the above mixture solution was sonicated for 30 min for establishing absorption-desorption equilibrium. A 1000 W xenon lamp was used as the light source, and placed at about 120 cm above of the mixture solution. The intensity of UV part between the wavelengths range of 320-400 nm was measured to be about 8 mW/cm2. The experiments were performed for 60 min, and samples were taken every other 10 min. The concentration of MB was monitored by measuring the absorbance of the supernatant at 665 nm using a UNICO UV-2102 spectrometer. A control test of MB photodegradation in absence of ZnO nanowires was also performed.
Results and discussion
Size uniformity is an important index to evaluate the quality of nanomaterials. Here, the size uniformity of the prepared ZnO nanowires was investigated by studying the diameter distribution of the nanowires. The diameters of the prepared ZnO nanowires were extracted from 200 nanowires in several SEM images. The diameter distribution histogram is shown in Figure 1c. It can be seen that the diameters of most of the nanowires ranged from 30 to 40 nm. The black solid line is the corresponding Gaussian line-fitting. It shows that the average diameter of these nanowires was about 33 nm.
The detailed microstructure of the ZnO nanowires was further characterized using TEM. Figure 1d shows a typical low-magnification TEM image of the prepared ZnO nanowires, revealing the representative morphology of the ZnO nanowires. It shows several straight and smooth nanowires with no secondary growth or extra structural features. Inset in Figure 1d shows a typical electron diffraction pattern of a single ZnO nanowire, suggesting the polycrystalline nature of the nanowires. An HRTEM image taken from a single nanowire is presented in Figure 1e. The clear lattice fringes in the HRTEM image indicate that the nanowire had a high degree of crystallinity and no amorphous materials existed at the interface. The lattice spacing is measured to be approximately 0.52 nm, which agrees well with the spacing of the (002) planes of the wurtzite ZnO structure. The TEM results suggest that the ZnO nanowires were structurally uniform polycrystalline nanowires.
In summary, we have demonstrated a rapid and catalyst-free technique for preparing large-scale ZnO nanowires. The technique is based on a modified carbothermal reduction method. ZnO nanowires prepared by this technique had a hexagonal wurtzite crystal structure, with an average diameter of 33.5 nm. Microstructure and optical properties characterization results indicated that the ZnO nanowires had a polycrystalline structure with a low concentration of oxygen vacancies. Photocatalytic activity evaluation measurements showed that the ZnO nanowires had a photodegradation rate constant of 1.86 h-1 to MB dye under UV irradiation.
This study was primarily supported by the National Nature Science Foundation of China Nos. 50730008, 50902092, and 61006002, and the Shanghai Science and Technology Grant No. 052nm02000 and 09JC1407400.
- Han F, Kambala VSR, Srinivasan M, Rajarathnam D, Naidu R: Tailored titanium dioxide photocatalysts for the degradation of organic dyes in wastewater treatment: a review. Appl Catal A: Gen 2009, 359: 25–40. 10.1016/j.apcata.2009.02.043View Article
- Yang L-Y, Dong S-Y, Sun J-H, Feng J-L, Wu Q-H, Sun S-P: Microwave-assisted preparation, characterization and photocatalytic properties of a dumbbell-shaped ZnO photocatalyst. J Hazard Mater 2010, 179: 438–443. 10.1016/j.jhazmat.2010.03.023View Article
- Zhang M, An T, Liu X, Hu X, Sheng G, Fu J: Preparation of a high-activity ZnO/TiO 2 photocatalyst via homogeneous hydrolysis method with low temperature crystallization. Mater Lett 2010, 64: 1883–1886. 10.1016/j.matlet.2010.05.054View Article
- Qu J, Luo C, Cong Q: Synthesis of multi-walled carbon nanotubes/ZnO nanocomposites using absorbent cotton. Nano-Micro Lett 2011, 3: 115–120.View Article
- Bao J, Shalish I, Su Z, Gurwitz R, Capasso F, Wang X, Ren Z: Photoinduced oxygen release and persistent photoconductivity in ZnO nanowires. Nanoscale Res Lett 2011, 6: 404. 10.1186/1556-276X-6-404View Article
- Chen H, Wu X, Gong L, Ye C, Qu F, Shen G: Hydrothermally grown ZnO micro/nanotube arrays and their properties. Nanoscale Res Lett 2010, 5: 570–575. 10.1007/s11671-009-9506-4View Article
- Zhang D, Chava S, Berven C, Lee SK, Devitt R, Katkanant V: Experimental study of electrical properties of ZnO nanowire random networks for gas sensing and electronic devices. Appl Phys A Mater 2010, 100: 145–150. 10.1007/s00339-010-5567-6View Article
- Zhu G, Yang R, Wang S, Wang ZL: Flexible high-output nanogenerator based on lateral ZnO nanowire array. Nano Lett 2010, 10: 3151–3155. 10.1021/nl101973hView Article
- Zhang Z, Meng GW, Xu QL, Hu YM, Wu Q, Hu Z: Aligned ZnO nanorods with tunable size and field emission on native Si substrate achieved via simple electrodeposition. J Phys Chem C 2010, 114: 189–193. 10.1021/jp9087223View Article
- Pauporté T, Bataille G, Joulaud L, Vermersch FJ: Well-aligned ZnO nanowire arrays prepared by seed-layer-free electrodeposition and their cassie-wenzel transition after hydrophobization. J Phys Chem C 2010, 114: 194–202. 10.1021/jp9087145View Article
- Mute A, Peres M, Peiris TC, Lourenço AC, Jensen LR, Monteiro T: Structural and optical characterization of ZnO nanowires grown on alumina by thermal evaporation method. J Nanosci Nanotechnol 2010, 10: 2669–2673. 10.1166/jnn.2010.1386View Article
- Hossain MF, Takahashi T: Microstructured ZnO photoelectrode grown on the sputter-deposited ZnO passivating-layer for improving the photovoltaic performances. Mater Chem Phys 124: 940–945.
- Fleischhaker F, Wloka V, Hennig I: ZnO based field-effect transistors (FETs): solution-processable at low temperatures on flexible substrates. J Mater Chem 2010, 20: 6622–6625. 10.1039/c0jm01477jView Article
- Park S-B, Kim B-G, Kim J-Y, Jung T-H, Lim D-G, Park J-H, Park J-G: Field-emission properties of patterned ZnO nanowires on 2.5D MEMS substrate. Appl Phys A Mater Sci Process 2010, 102: 169–172.View Article
- Choi A, Kim K, Jung HI, Lee SY: ZnO nanowire biosensors for detection of biomolecular interactions in enhancement mode. Sensor Actuat B Chem 2010, 148: 577–582. 10.1016/j.snb.2010.04.049View Article
- Umar A, Karunagaran B, Suh E-K, Hahn YB: Structural and optical properties of single-crystalline ZnO nanorods grown on silicon by thermal evaporation. Nanotechnology 2006, 17: 4072. 10.1088/0957-4484/17/16/013View Article
- Alim KA, Fonoberov VA, Balandin AA: Origin of the optical phonon frequency shifts in ZnO quantum dots. Appl Phys Lett 2005, 86: 053103. 10.1063/1.1861509View Article
- Kim HW, Kebede MA, Kim HS: Structural, Raman, and photoluminescence characteristics of ZnO nanowires coated with Al-doped ZnO shell layers. Curr Appl Phys 2010, 10: 60–63. 10.1016/j.cap.2009.04.012View Article
- Tzolov M, Tzenov N, Dimova-Malinovska D, Kalitzova M, Pizzuto C, Vitali G, Zollo G, Ivanov I: Vibrational properties and structure of undoped and Al-doped ZnO films deposited by RF magnetron sputtering. Thin Solid Films 2000, 379: 28–36. 10.1016/S0040-6090(00)01413-9View Article
- Greyson E, Babayan Y, Odom T: Directed growth of ordered arrays of small-diameter ZnO nanowires. Adv Mater 2004, 16: 1348–1352. 10.1002/adma.200400765View Article
- Vanheusden K, Warren WL, Seager CH, Tallant DR, Voigt JA, Gnade BE: Mechanisms behind green photoluminescence in ZnO phosphor powders. J Appl Phys 1996, 79: 7983–7990. 10.1063/1.362349View Article
- Mekasuwandumrong O, Pawinrat P, Praserthdam P, Panpranot J: Effects of synthesis conditions and annealing post-treatment on the photocatalytic activities of ZnO nanoparticles in the degradation of methylene blue dye. Chem Eng J 2010, 164: 77–84. 10.1016/j.cej.2010.08.027View Article
- Xie W, Li Y, Sun W, Huang J, Xie H, Zhao X: Surface modification of ZnO with Ag improves its photocatalytic efficiency and photostability. J Photochem Photobiol A 2010, 216: 149–155. 10.1016/j.jphotochem.2010.06.032View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.